LMucko/crystallography-open-database huggingface dataset:
Magnetic structure versus electron number for some rare-earth intermetallic compounds
Koehler, W.C.; Child, H.R.; Cable, J.W.; Journal of Applied Physics 36 (1965) 1096–1097; doi:10.1063/1.1714115

data_1508987
_publ_section_title
;
 Magnetic structure versus electron number for some rare-earth
 intermetallic compounds
;
_journal_name_full               'Journal of Applied Physics'
_journal_page_first              1096
_journal_page_last               1097
_journal_paper_doi               10.1063/1.1714115
_journal_volume                  36
_journal_year                    1965
_chemical_formula_sum            'Ag0.5 In0.5 Tb'
_chemical_name_systematic        'Silver terbium indium (0.5/1/0.5)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.68
_cell_length_b                   3.68
_cell_length_c                   3.68
_cell_volume                     49.836
_citation_journal_id_ASTM        JAPIAU
_cod_data_source_file            silver0-1_112.cif
_cod_data_source_block           Ag0.5In0.5Tb1
_cod_original_cell_volume        49.83603
_cod_original_formula_sum        'Ag0.5 In0.5 Tb1'
_cod_database_code               1508987
Magnetic and structural studies of the alloy system RE In0.5 Ag0.5
Methfessel, S.; Lal, H.B.; Journal of Magnetism and Magnetic Materials 23 (1981) 283–290; doi:10.1016/0304-8853(81)90049-4

data_1508988
_publ_section_title
;
 Magnetic and structural studies of the alloy system RE In0.5 Ag0.5
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              283
_journal_page_last               290
_journal_paper_doi               10.1016/0304-8853(81)90049-4
_journal_volume                  23
_journal_year                    1981
_chemical_formula_sum            'Ag0.5 In0.5 Tb'
_chemical_name_systematic        'Silver indium terbium (0.5/0.5/1)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.702
_cell_length_b                   3.702
_cell_length_c                   3.702
_cell_volume                     50.735
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            silver0-1_113.cif
_cod_data_source_block           Ag0.5In0.5Tb1
_cod_original_cell_volume        50.73518
_cod_original_formula_sum        'Ag0.5 In0.5 Tb1'
_cod_database_code               1508988
Magnetic and structural studies of the alloy system RE In0.5 Ag0.5
Lal, H.B.; Methfessel, S.; Journal of Magnetism and Magnetic Materials 23 (1981) 283–290; doi:10.1016/0304-8853(81)90049-4

data_1508989
_publ_section_title
;
 Magnetic and structural studies of the alloy system RE In0.5 Ag0.5
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              283
_journal_page_last               290
_journal_paper_doi               10.1016/0304-8853(81)90049-4
_journal_volume                  23
_journal_year                    1981
_chemical_formula_sum            'Ag0.5 In0.5 Tm'
_chemical_name_systematic        'Silver indium thulium (0.5/0.5/1)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.629
_cell_length_b                   3.629
_cell_length_c                   3.629
_cell_volume                     47.793
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            silver0-1_114.cif
_cod_data_source_block           Ag0.5In0.5Tm1
_cod_original_cell_volume        47.79263
_cod_original_formula_sum        'Ag0.5 In0.5 Tm1'
_cod_database_code               1508989
Thermal and X-ray investigations of the quasi-binary system Ag1-x Pdx Mg (x=0-0.5)
Sharma, S.N.; Weiss, A.; Journal of the Less-Common Metals 104 (1984) L5–L8; doi:10.1016/0022-5088(84)90459-4

data_1508990
_publ_section_title
;
 Thermal and X-ray investigations of the quasi-binary system Ag1-x Pdx Mg
 (x=0-0.5)
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              L5
_journal_page_last               L8
_journal_paper_doi               10.1016/0022-5088(84)90459-4
_journal_volume                  104
_journal_year                    1984
_chemical_formula_sum            'Ag0.5 Mg Pd0.5'
_chemical_name_systematic        'Silver palladium magnesium (0.5/0.5/1)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.239
_cell_length_b                   3.239
_cell_length_c                   3.239
_cell_volume                     33.981
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver0-1_115.cif
_cod_data_source_block           Ag0.5Mg1Pd0.5
_cod_original_cell_volume        33.98074
_cod_original_formula_sum        'Ag0.5 Mg1 Pd0.5'
_cod_database_code               1508990
Crystal structure of Ag2 Te S3 and Na (Na1-x Agx) Te S3 (x = 0.5) and the geometry of Te(IV) S3 polyhedra
Pertlik, F.; Monatshefte fuer Chemie und verwandte Teile anderer Wissenschaften (109,1978-) 128 (1997) 157–163; doi:

data_1508991
_publ_section_title
;
 Crystal structure of Ag2 Te S3 and Na (Na1-x Agx) Te S3 (x = 0.5) and the
 geometry of Te(IV) S3 polyhedra
;
_journal_name_full
;
Monatshefte fuer Chemie und verwandte Teile anderer Wissenschaften (109,1978-)
;
_journal_page_first              157
_journal_page_last               163
_journal_volume                  128
_journal_year                    1997
_chemical_formula_sum            'Ag0.5 Na1.5 S3 Te'
_chemical_name_systematic
'Sodium silver tellurium sulfide (1.5/0.5/1/3)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 92.26
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.761
_cell_length_b                   12.171
_cell_length_c                   8.342
_cell_volume                     584.462
_citation_journal_id_ASTM        MOCMB7
_cod_data_source_file            silver0-1_116.cif
_cod_data_source_block           Ag0.5Na1.5S3Te1
_cod_original_cell_volume        584.4622
_cod_original_formula_sum        'Ag0.5 Na1.5 S3 Te1'
_cod_database_code               1508991
Crystal structure of the compound Nd5 Ag0.5 Si3.5
Zaplatynsky, O.V.; Stepen'-Damm, Yu.; Salamakha, P.S.; Prots', Yu.M.; Bodak, O.I.; Journal of Alloys Compd. 221 (1995) 91–93; doi:10.1016/0925-8388(94)01379-9

data_1508992
_publ_section_title
;
 Crystal structure of the compound Nd5 Ag0.5 Si3.5
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              91
_journal_page_last               93
_journal_paper_doi               10.1016/0925-8388(94)01379-9
_journal_volume                  221
_journal_year                    1995
_chemical_formula_sum            'Ag0.5 Nd5 Si3.5'
_chemical_name_systematic        'Neodymium argentide silicide (5/0.5/3.5)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.645
_cell_length_b                   15.04
_cell_length_c                   7.881
_cell_volume                     906.164
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            silver0-1_117.cif
_cod_data_source_block           Ag0.5Nd5Si3.5
_cod_original_cell_volume        906.1637
_cod_database_code               1508992
Magnetic structure versus electron number for some rare-earth intermetallic compounds
Cable, J.W.; Koehler, W.C.; Child, J.R.; Journal of Applied Physics 36 (1965) 1096–1097; doi:10.1063/1.1714115

data_1508993
_publ_section_title
;
 Magnetic structure versus electron number for some rare-earth
 intermetallic compounds
;
_journal_name_full               'Journal of Applied Physics'
_journal_page_first              1096
_journal_page_last               1097
_journal_paper_doi               10.1063/1.1714115
_journal_volume                  36
_journal_year                    1965
_chemical_formula_sum            'Ag0.5 Pd0.5 Tb'
_chemical_name_systematic        'Silver palladium terbium (0.5/0.5/1)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.54
_cell_length_b                   3.54
_cell_length_c                   3.54
_cell_volume                     44.362
_citation_journal_id_ASTM        JAPIAU
_cod_data_source_file            silver0-1_119.cif
_cod_data_source_block           Ag0.5Pd0.5Tb1
_cod_original_cell_volume        44.36186
_cod_original_formula_sum        'Ag0.5 Pd0.5 Tb1'
_cod_database_code               1508993
The atomic arrangements and bonds of the gold-silver ditellurides
Pauling, L.; Tunell, G.; Acta Crystallographica (1,1948-23,1967) 5 (1952) 375–381; doi:10.1107/S0365110X52001106

data_2310019
_publ_section_title
;
 The atomic arrangements and bonds of the gold-silver ditellurides
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              375
_journal_page_last               381
_journal_paper_doi               10.1107/S0365110X52001106
_journal_volume                  5
_journal_year                    1952
_chemical_formula_sum            'Ag0.1 Au0.9 Te2'
_chemical_name_systematic        'Gold silver telluride (0.9/0.1/2)'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.22
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.19
_cell_length_b                   4.4
_cell_length_c                   5.07
_cell_volume                     160.393
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            silver0-1_12.cif
_cod_data_source_block           Ag0.1Au0.9Te2
_cod_original_cell_volume        160.3933
_cod_database_code               2310019
Magnetic properties of Tb Ag1-x Znx solid solutions
Chechernikov, V.I.; Tavansi, A.; Kurenchanin, V.V.; Sinanyan, L.G.; Fizika Metallov i Metallovedenie 43 (1977) 155–157; doi:

data_1508994
_publ_section_title
;
 Magnetic properties of Tb Ag1-x Znx solid solutions
;
_journal_name_full               'Fizika Metallov i Metallovedenie'
_journal_page_first              155
_journal_page_last               157
_journal_volume                  43
_journal_year                    1977
_chemical_formula_sum            'Ag0.5 Tb Zn0.5'
_chemical_name_systematic        'Silver zinc terbium (0.5/0.5/1)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.595
_cell_length_b                   3.595
_cell_length_c                   3.595
_cell_volume                     46.462
_citation_journal_id_ASTM        FMMTAK
_cod_data_source_file            silver0-1_120.cif
_cod_data_source_block           Ag0.5Tb1Zn0.5
_cod_original_cell_volume        46.46187
_cod_original_formula_sum        'Ag0.5 Tb1 Zn0.5'
_cod_database_code               1508994
Lattice spacing ralationships in hexagonal close-packed silver-zinc-manganese alloys
Wilcox, R.J.M.; Henderson, B.; Philosophical Magazine, Serie 8(1956-) 9 (1964) 829–846; doi:

data_1508995
_publ_section_title
;
 Lattice spacing ralationships in hexagonal close-packed
 silver-zinc-manganese alloys
;
_journal_name_full               'Philosophical Magazine, Serie 8(1956-)'
_journal_page_first              829
_journal_page_last               846
_journal_volume                  9
_journal_year                    1964
_chemical_formula_sum            'Ag0.5 Zn1.5'
_chemical_name_systematic        'Silver zinc (0.5/1.5)'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.8231
_cell_length_b                   2.8231
_cell_length_c                   4.4407
_cell_volume                     30.650
_citation_journal_id_ASTM        PHMA83
_cod_data_source_file            silver0-1_121.cif
_cod_data_source_block           Ag0.5Zn1.5
_cod_original_cell_volume        30.65029
_cod_database_code               1508995
Phase diagram of the (Ag Ga Se2) - (Cd Se) system and crystal structure of the Ag Cd2 Ga Se4 compound
Olekseyuk, I.D.; Husak, O.A.; Gulay, L.D.; Kadykalo, E.M.; Parasyuk, O.V.; Journal of Alloys Compd. 343 (2002) 125–131; doi:10.1016/S0925-8388(02)00143-3

data_1508996
_publ_section_title
;
 Phase diagram of the (Ag Ga Se2) - (Cd Se) system and crystal structure
 of the Ag Cd2 Ga Se4 compound
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              125
_journal_page_last               131
_journal_paper_doi               10.1016/S0925-8388(02)00143-3
_journal_volume                  343
_journal_year                    2002
_chemical_formula_sum            'Ag0.52 Cd0.96 Ga0.52 Se2'
_chemical_name_systematic
'Silver cadmium gallium selenide (0.52/0.96/0.52/2)'
_space_group_IT_number           186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   4.2088
_cell_length_b                   4.2088
_cell_length_c                   6.8956
_cell_volume                     105.784
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            silver0-1_122.cif
_cod_data_source_block           Ag0.52Cd0.96Ga0.52Se2
_cod_original_cell_volume        105.7838
_cod_database_code               1508996
Phase equilibria and the crystal structure of compounds in the (Ti, Hf) - Ag - Ga systems
Verbovits'kii, Yu.V.; Kotur, B.Ya.; Dopov. Nats. Akad. Nauk. Ukr. 2003 (2003) 132–136; doi:

data_1508997
_publ_section_title
;
 Phase equilibria and the crystal structure of compounds in the (Ti, Hf) -
 Ag - Ga systems
;
_journal_name_full               'Dopov. Nats. Akad. Nauk. Ukr.'
_journal_page_first              132
_journal_page_last               136
_journal_volume                  2003
_journal_year                    2003
_chemical_formula_sum            'Ag0.52 Ga2.48 Ti'
_chemical_name_systematic        'Titanium silver gallium (1/0.52/2.48)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.984
_cell_length_b                   3.984
_cell_length_c                   3.984
_cell_volume                     63.235
_citation_journal_id_ASTM        DNAUFL
_cod_data_source_file            silver0-1_123.cif
_cod_data_source_block           Ag0.52Ga2.48Ti1
_cod_original_cell_volume        63.23507
_cod_original_formula_sum        'Ag0.52 Ga2.48 Ti1'
_cod_database_code               1508997
Effect of deformation and low temperatures on the structures of Ag Cd and Au Zn
Masson, D.B.; Barrett, C.S.; Transactions of the Metallurgical Society of Aime 212 (1958) 260–265; doi:

data_1508998
_publ_section_title
;
 Effect of deformation and low temperatures on the structures of Ag Cd and
 Au Zn
;
_journal_name_full
'Transactions of the Metallurgical Society of Aime'
_journal_page_first              260
_journal_page_last               265
_journal_volume                  212
_journal_year                    1958
_chemical_formula_sum            'Ag0.53 Cd0.47'
_chemical_name_systematic        'Silver cadmium (0.53/0.47) - LT'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.116
_cell_length_b                   4.89
_cell_length_c                   4.779
_cell_volume                     72.819
_citation_journal_id_ASTM        TMSAAB
_cod_data_source_file            silver0-1_124.cif
_cod_data_source_block           Ag0.53Cd0.47
_cod_original_cell_volume        72.81876
_cod_database_code               1508998
Neue ternaere Vertreter des Th Cr2 Si2- und des Ca Zn2 Al2-Strukturtyps in den Systemen A-T-X und RE-T-X (A= Ca, Sr, Ca; RE= La, Ce, Pr; T= Cu, Ag, Au und X= Al,Ga).
Doersam, G.; Roehr, C.; Cordier, G.; Journal of the Less-Common Metals 166 (1990) 115–124; doi:10.1016/0022-5088(90)90371-P

data_1508999
_publ_section_title
;
 Neue ternaere Vertreter des Th Cr2 Si2- und des Ca Zn2 Al2-Strukturtyps
 in den Systemen A-T-X und RE-T-X (A= Ca, Sr, Ca; RE= La, Ce, Pr; T= Cu,
 Ag, Au und X= Al,Ga).
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              115
_journal_page_last               124
_journal_paper_doi               10.1016/0022-5088(90)90371-P
_journal_volume                  166
_journal_year                    1990
_chemical_formula_sum            'Ag0.57 Ga3.43 Sr'
_chemical_name_systematic        'Strontium silver gallium (1/0.57/3.43)'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.405
_cell_length_b                   4.405
_cell_length_c                   10.914
_cell_volume                     211.776
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver0-1_125.cif
_cod_data_source_block           Ag0.57Ga3.43Sr1
_cod_original_cell_volume        211.7755
_cod_original_formula_sum        'Ag0.57 Ga3.43 Sr1'
_cod_database_code               1508999
Constitution, structural chemistry and magnetism in the ternary system Ce - Ag- Si
Saccone, A.; Cordruwisch, E.; Ferro, R.; Rogl, P.; Kaczorowski, D.; Journal of Alloys Compd. 320 (2001) 308–319; doi:10.1016/S0925-8388(00)01474-2

data_1509000
_publ_section_title
;
 Constitution, structural chemistry and magnetism in the ternary system Ce
 - Ag- Si
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              308
_journal_page_last               319
_journal_paper_doi               10.1016/S0925-8388(00)01474-2
_journal_volume                  320
_journal_year                    2001
_chemical_formula_sum            'Ag0.5728 Ce Si1.2172'
_chemical_name_systematic        'Cerium silver silicide (1/0.57/1.22)'
_space_group_IT_number           191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   4.2732
_cell_length_b                   4.2732
_cell_length_c                   4.2012
_cell_volume                     66.437
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            silver0-1_126.cif
_cod_data_source_block           Ag0.5728Ce1Si1.2172
_cod_original_cell_volume        66.43707
_cod_original_formula_sum        'Ag0.5728 Ce1 Si1.2172'
_cod_database_code               1509000
Constitution, structural chemistry and magnetism in the ternary system Ce - Ag- Si
Ferro, R.; Saccone, A.; Kaczorowski, D.; Rogl, P.; Cordruwisch, E.; Journal of Alloys Compd. 320 (2001) 308–319; doi:10.1016/S0925-8388(00)01474-2

data_1509001
_publ_section_title
;
 Constitution, structural chemistry and magnetism in the ternary system Ce
 - Ag- Si
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              308
_journal_page_last               319
_journal_paper_doi               10.1016/S0925-8388(00)01474-2
_journal_volume                  320
_journal_year                    2001
_chemical_formula_sum            'Ag0.58 Ce Si1.42'
_chemical_name_systematic        'Cerium silver silicide (1/0.58/1.42)'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.2291
_cell_length_b                   4.2291
_cell_length_c                   14.6374
_cell_volume                     261.794
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            silver0-1_127.cif
_cod_data_source_block           Ag0.58Ce1Si1.42
_cod_original_cell_volume        261.7941
_cod_original_formula_sum        'Ag0.58 Ce1 Si1.42'
_cod_database_code               1509001
Crystal structure of lanthanum silver aluminium, LaAg0.6Al3.4
Cordier, G.; Doersam, G.; Dietrich, C.; Zeitschrift fuer Kristallographie - New Crystal Structures 212 (1997) 288–288; doi:

data_8103383
_publ_section_title
;
 Crystal structure of lanthanum silver aluminium, LaAg0.6Al3.4
;
_journal_name_full
;
Zeitschrift fuer Kristallographie - New Crystal Structures
;
_journal_page_first              288
_journal_page_last               288
_journal_volume                  212
_journal_year                    1997
_chemical_formula_sum            'Ag0.553 Al3.447 La'
_chemical_name_systematic        'Silver aluminium lanthanum (0.6/3.4/1)'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.18
_cell_length_b                   6.18
_cell_length_c                   11.051
_cell_volume                     422.064
_citation_journal_id_ASTM        ZKNSFT
_cod_data_source_file            silver0-1_128.cif
_cod_data_source_block           Ag0.553Al3.447La1
_cod_original_cell_volume        422.0642
_cod_original_formula_sum        'Ag0.553 Al3.447 La1'
_cod_database_code               8103383